Lasers Med Sci (2012) 27:145–151DOI 10.1007/s10103-010-0857-y ORIGINAL ARTICLEThe effect of curing light and chemical catalyst on the degreeof conversion of two dual cured resin luting cementsEduardo José Souza-Junior & Lúcia Trazzi Prieto & Giulliana Panfiglio Soares &Carlos Tadeu dos Santos Dias & Flávio Henrique Baggio Aguiar &Luís Alexandre Maffei Sartini PaulilloReceived: 31 March 2010 / Accepted: 28 October 2010 / Published online: 23 November 2010# Springer-Verlag London Ltd 2010Abstract The aim of this study was to evaluate the of the use of the chemical catalyst and light curing source.influence of different curing lights and chemical catalysts In conclusion, RelyX ARC can be cured satisfactorily withon the degree of conversion of resin luting cements. A total the argon ion laser, LED or quartz-tungsten-halogen lightof 60 disk-shaped specimens of RelyX ARC or Panavia F with or without a chemical catalyst. To obtain a satisfactoryof diameter 5 mm and thickness 0.5 mm were prepared and degree of conversion, Panavia F luting cement should bethe respective chemical catalyst (Scotchbond Multi-Purpose used with ED Primer and cured with halogen light.Plus or ED Primer) was added. The specimens were light-cured using different curing units (an argon ion laser, an Keywords Curing light . Degree of cure . Resin cement .LED or a quartz-tungsten-halogen light) through shade A2 Photoactivationcomposite disks of diameter 10 mm and thickness 2 mm.After 24 h of dry storage at 37°C, the degree of conversionof the resin luting cements was measured by Fourier- Introductiontransformed infrared spectroscopy. For statistical analysis,ANOVA and the Tukey test were used, with p≤0.05. With the new developments in adhesive dentistry, resin lutingPanavia F when used without catalyst and cured using the cements have become widely used due to their ability to bondLED or the argon ion laser showed degree of conversion indirect restorations to the tooth structure [1, 2]. Thesevalues significantly lower than RelyX ARC, with and materials can minimize some adverse effects of directwithout catalyst, and cured with any of the light sources. composite restorations, such as polymerization contractionTherefore, the degree of conversion of Panavia F with ED stress  and gap formation at the tooth/restoration interfacePrimer cured with the quartz-tungsten-halogen light was . Therefore, the procedure involving resinous luting ofsignificantly different from that of RelyX ARC regardless thick and opaque indirect restorations and fiber posts needs an adequate cure to reach a satisfactory degree of conversion of the cement used [2, 5]. The degree of conversion isE. J. Souza-Junior (*) : L. T. Prieto affected by the attenuation of the light that reaches the resinPiracicaba Dental School, Department of Restorative Dentistry, cement, by the distance of the light source tip, irradiance andUniversity of Campinas - UNICAMP,P.O. Box 52, Avenida Limeira, 901, Areião, energy density applied, and by the transmission properties of13414-903, Piracicaba, SP, Brazil the indirect restoration . An insufficient degree ofe-mail: email@example.com conversion can lead to deficient mechanical properties ofG. P. Soares : F. H. B. Aguiar : L. A. M. S. Paulillo the resin luting cement, including inadequate hardness [6, 7],Piracicaba Dental School, Department of Restorative Dentistry, wear resistance  and water sorption, residual monomerState University of Campinas – UNICAMP, , and problems with biocompatibility. A low degree ofPiracicaba, SP, Brazil resin polymerization increases the risk of restoration failure and marginal fracture, gap formation and the occurrence ofC. T. dos Santos DiasDepartment of Exact Science, University of São Paulo, secondary caries , and reduces the retention of the indirectSão Paulo, Brazil restoration or the post .
146 Lasers Med Sci (2012) 27:145–151 In an attempt to overcome these problems, dual curing chemical catalyst on cement manipulation and differentresin cements were developed to combine important light curing units on the degree of conversion of resin lutingproperties of chemical-cured and light-cured materials so cements.as to provide efficient cure in deeper areas and places withreduced light penetration [2, 11]. However, in somesituations, the polymerization reaction may be mainly Materials and methodsactivated by a chemical mechanism (self-cure). Chemicalcatalysts have been used with luting materials with the aim Experimental designof promoting better resin cement properties . Thesecatalyst formulations contain coinitiator systems, such as The dual cured resin luting cement Panavia F (Kuraraytertiary amine/benzoyl peroxide, that may improve the rate Medical, Tokyo, Japan) and RelyX ARC (3 M ESPE, St.of monomer conversion when mixed with the material, Paul, MN), with their respective chemical catalysts incor-especially in regions with poor light penetration . porated by manipulation of the material, were tested. The On the other hand, choosing the correct light source for composition of the materials is shown in Table 1. A total ofcuring is important to achieve a satisfactory degree of cure 60 disk-shaped specimens of diameter 5 mm and thicknessof the resin luting cement. Traditionally, quartz-tungsten- 0.5 mm were prepared from the resin cements using thehalogen (QTH) lights have been widely used in dental respective chemical catalysts. For specimen preparation, thepractice. They have a spectral wavelength in the range 400– cements were placed in a silicon mold (Express XT; 3 M500 nm and an irradiance in the range 300–1,000 mW/cm2 ESPE, St Paul, MN) and then covered with Mylar film and[12, 13]. However, they have some drawbacks, such as a glass slide, in order to form a flat surface.gradual reduction in irradiance over time, the need for For Panavia F alone, equal amounts (27 g) of base andfilters for wavelength selection, limited depth of cure, and catalyst were weighed on an analytical balance , mixedconsiderable heat generation [14, 15]. Blue light emitting for 15 s, and then immediately photocured. In the groups todiode (LED) units have a narrow spectral range, which which the ED Primer had been added, one drop of each oftargets the absorption wavelength of camphorquinone, with the primer liquids A and B was mixed for 10 s, and gentlya peak value of 468 nm, allowing low amounts of wasted air-dried for 5 s for solvent evaporation. Thereafter, 1.4 mgenergy and minimum heat generation [14, 16]. It has been of this solution was mixed with equal amounts (27 g) ofclaimed that this could provide higher monomer conversion base and catalyst of Panavia F for 15 s, and immediatelyefficiency and reduce the exposure time required . photocured .Studies have shown that current LED curing units can Specimens of RelyX ARC alone were prepared in the samereplace, in most situations, conventional QTH light units way as the Panavia F specimens, with equal amounts (27 g) of[15, 18]. base and catalyst, mixed for 15 s and then photocured. For The argon ion laser has arisen as an alternative light specimens with the added chemical catalyst (catalyst ofsource for polymerizing resin composites, resin luting Scotchbond Multi-Purpose), 1.4 mg of the liquid was mixedcements, and for bleaching procedures [19–21]. For with equal amounts (27 g) of base and catalyst of RelyX ARCcamphorquinone-based resins, the activation emits a blue for 15 s, and immediately photocured.light in the wavelength range 400–500 nm with peak values A disk (10 mm in diameter and 2 mm thick) of aat about 468 and 480 nm, depending on the monomer nanofilled resin composite shade A2 (Filtek Z350; 3 Mformulation, and it has an irradiance at up to 2,000 mW/cm2 ESPE) was prepared to simulate an indirect restoration. The[21–24]. Furthermore, the argon ion laser has certain resin luting cements were light-cured through the compositecharacteristics, such as low beam divergence, collimation, for 40 s, using three light sources: argon ion laser atmonochromaticity, coherency, absorption selectivity and 600 mW/cm 2 (Accucure 3000/Lasermed); LED atfiber delivery ability, that make it particularly suitable for 1,400 mW/cm2 (FLASHlite 1401/Discus Dental); andclinical use to cure resinous materials with a greater degree QTH light at 600 mW/cm2 (VIP/Bisco, Schaumburg, IL).of cure and improved physical and mechanical properties The irradiance of all curing sources was measured with a[22, 23, 25]. Although these laser units may accelerate the radiometer before light activation (Demetron Kerr Corpo-cure of composites, they can promote a temperature increase ration, Orange, CA). The light spectra of all curing units areat the light-curing tip . shown in Fig. 1. The effect of the chemical catalyst on the properties ofresin luting cements has not yet been clarified. Also, Degree of conversiondetermining the most effective light source for curing resincements still needs more study. Therefore, the aim of this After 24 hours of dry storage at 37°C in the dark, thestudy was to evaluate the influence of the incorporation of a degree of conversion (DC) of the specimens was deter-
Lasers Med Sci (2012) 27:145–151 147Table 1 Materials used in the study with composition and manufacturer’s informationResin cements Composition ManufacturerPanavia F Paste A (batch 00250B): 10-Methacryloyloxydecyl dihydrogen phosphate, Kuraray Medical, hydrophobic aromatic dimethacrylate, hydrophobic aliphatic dimethacrylate, Tokyo, Japan hydrophilic dimethacrylate, silanated sílica, photoinitiators, DL-camphorquinone, benzoyl peroxide Paste B (batch 00027B): Hydrophobic aromatic dimethacrylate, hydrophobic aliphatic dimethacrylate, hydrophilic dimethacrylate. Sodium aromatic sulfinate, accelerator, sodium fluoride, silanated barium glassED Primer Primer A (batch 00272A): 2-Hydroxyethyl methacrylate, methacryloyloxydecyl Kuraray Medical, dihydrogen phosphate, NM-aminosalicylic acid, diethanol-p-toluidine, water Tokyo, Japan Primer B (batch 00147A): NM-Aminosalicylic acid, T-isopropylic benzenic sodium sulfinate, diethanol-p-toluidine, waterRelyX ARC (batch GU9JG) Paste A: Silane-treated ceramic, bis-glycidyl methacrylate, triethylene glycol dimethacrylate, 3 M ESPE, photoinitiators, amine, silane-treated silica, functionalized dimethacrylate polymer St Paul, MN Paste B: Silane-treated ceramic, triethylene glycol dimethacrylate, bis-glycidyl methacrylate, silane-treated silica, benzoyl peroxide, functionalized dimethacrylate polymerCatalyst for Scotchbond Bisphenol A diglycidyl ether dimethacrylate, 2-hydroxyethyl methacrylate, benzoyl peroxide 3 M ESPE, Multi-Purpose (batch 9BE) St Paul, MNmined using Fourier transform infrared spectroscopy A one-way ANOVA was performed to compare the(FTIR) with a Spectrum 100 instrument (PerkinElmer, differences among the tested groups at a preset alpha ofShelton, CT). For each specimen 32 spectra were analyzed. 0.05, followed by Tukey’s post hoc test.The ratio between the intensities of aliphatic C=C (at1,637.3 cm−1) and aromatic C=C (at 1,608.3 cm−1) peaksfor uncured and cured samples were used to calculate the Resultsdegree of conversion, according to the following equation: Means and standard deviations of the degree of conversion ½Abs ðC ¼ C aliphÞ=Abs ðC::: C aromÞ cured resinDC ¼ 1 À ::: of the resin luting cements are shown in Table 2. Panavia F ½Abs ðC ¼ C aliphÞ=AbsðC C aromÞ uncured risen photocured with the LED and with the argon ion laser Â 100 without chemical catalyst exhibited the lowest degree ofwhere DC is the degree of conversion, Abs(C=C arom) is conversion, which was significantly different from that ofthe height of the benzene ring peak, and Abs(C=C aliph) is the other groups tested (p≤0.05). For the RelyX lutingthe height of the aliphatic C=C bond peak, for both cured cement, no statistically significant differences in the degreeand uncured composites. of conversion were found between the light sources and the presence of chemical catalyst on manipulation. Photo- polymerization with the QTH light showed better degree of conversion, which was significantly different from the degree of conversion with the LED and with the laser for Panavia F without catalyst incorporation. However, for RelyX ARC alone, there were no differences between the degrees of conversion achieved with any of the light curing units (p≥0.05). Figures 2 and 3 show the means of the degrees of conversion for Panavia F and RelyX ARC. Discussion The resin luting cements used in this study (RelyX ARC and Panavia F) are widely used in clinical practice for cementing fiber posts and indirect restorations. Most resin luting materials contain a diketone photoinitiator, such asFig. 1 Spectra of the light curing units used camphorquinone with a broad absorption spectral peak at
148 Lasers Med Sci (2012) 27:145–151Table 2 Degrees of (percentage) conversion of the tested groups.Values are means (standard deviations)Group Degree of conversion (%)1. RelyX ARC+LED 68.68 (9.10) A2. RelyX ARC+Laser+catalyst 67.58 (5.84) A3. RelyX ARC+LED+catalyst 62.0 (4.73) AB4. RelyX ARC+Laser 60.4 (10.1) AB5. RelyX ARC+QTH 59.2 (11.3) AB6. RelyX ARC+QTH+catalyst 54.26 (5.84) ABC7. Panavia F+QTH+catalyst 54.1 (5.61) ABC8. Panavia F+QTH 44.9 (9.49) BC Fig. 3 Degrees of conversion (means±SD) for RelyX ARC9. Panavia F+LED+catalyst 42.0 (6.23) BC10. Panavia F+Laser+catalyst 35.6 (3.07) C11. Panavia F+LED 10.91(8.68) D 54.1%) when QTH light was used, regardless of the12. Panavia F+Laser 7.10 (5.53) D incorporation of ED Primer. The results suggest that RelyX ARC may contain camphorquinone in a higher percentageDifferent letters mean statistical significant difference among the groups than Panavia F, since the curing units with a narrower spectrum range for the absorption peak of this photo-468 nm in the blue region of the visible spectrum [26, 27]. initiator (the LED and the argon ion laser) did not influenceHowever, the spectral distribution of the output from the monomer conversion, compared to the QTH curing light.curing light source and the maximum absorption peak of a Therefore, Panavia F, when cured with the LED and thephotoinitiator can affect the chemical and physical properties laser without ED Primer incorporation, reached a poorof a given resin. degree of conversion in comparison with that achieved with Some resinous photocure or dual cure materials, such as the QTH light. Thus, ED Primer should be incorporatedresin cements, may have a lower concentration of cam- with Panavia F in any manipulation procedure in order tophorquinone or other photoinitiator such as phenyl pro- achieve a satisfactory degree of monomer conversion and,panedione  (PPD) and monoacrylphosphine oxide  consequently, clinical success.(TPO), and sometimes the percentage of photoinitiator is Faria-e-Silva et al.  found that the degree of conversionnot clarified by the manufacturer because a patent on the of Panavia F was approximately 60% when photocured withproduct has been applied for. For Panavia F, the manufac- halogen light under a resin composite disk. In this study, theturer omits the percentage of the camphorquinone-based highest degree of conversion of Panavia F was 54.1% whenphotoinitiator system, and the percentage and composition used with the chemical catalyst and cured with the QTHof the photoinitiator component for RelyX ARC is light. However, other authors  have stated that whenunknown. The degree of conversion of RelyX ARC was cured directly with a LED, this cement reaches about 48%not influenced by either the curing light or chemical monomer conversion; however, in this study when thiscatalyst (54.26% to 68.68%); however, Panavia F just cement was cured with the LED unit under a resin compositereached an adequate monomer conversion rate (44.9% and disk, the degree of conversion reached about 10.91%, which is unsatisfactory for clinical applications. The curing units used in this work emitted different irradiances and final energy densities after 40 s for photo- activation was adopted for all light sources (QTH and laser, 600 mW/cm2 and 24 J; LED, 1,200 mW/cm2 and 48 J). Although higher values of irradiance induce greater heat generation, the composite disk attenuated the temperature alteration caused by the LED since the composite had a low thermal conductivity [27, 29], and did not affect the degree of conversion of the tested resin cements. The curing unit energy density did not influence the degree of conversion of Panavia F cured without ED primer, since QTH provided a significantly higher degree of conversion than the LED when ED Primer was not used. This finding may be associatedFig. 2 Degrees of conversion (means±SD) for Panavia F (*p0.05) with the photoinitiator content of Panavia F and the broad
Lasers Med Sci (2012) 27:145–151 149spectral range of QTH light that can reach alternative curing can occur and such a delay does not stop thephotoinitiators better than the second-generation LED used conversion of monomers by the free radical polymerizationin this study, even though the latter emits a higher irradiance center . In this study specimens were immediatelyfor the same curing time than the QTH light. For photocured for the sake of standardization because theconventional camphorquinone-based resin composites, no manufacturers of some resin luting cements do notdifference has been observed in the development of physical recommend such a delay in photoactivation.properties, such as the degree of conversion, when LED and The chemical catalysts used in this study containedQTH units are compared [13, 31]. benzoyl peroxide, which might be able to start some The argon ion laser has been described as a promising chemical cure at the material matrix . The self-cure islight source for curing resinous materials . In spite of initiated with a reaction between benzoyl peroxide andsome benefits, such as an economic benefit of 25–33%, tertiary amine that releases free radicals which promoteadequate depth of cure, and enhancement in resin physical monomer conversion regardless of exposure to light curingproperties after polymerization, the laser absorption peak is . Thus, the catalyst of the Scotchbond Multi-Purposeat 488 nm, displacing the camphorquinone absorption peak system contains only benzoyl peroxide as an initiatorat 468 nm [32, 33]. In some situations, this distance can system. This catalyst did not influence the degree of curemake activation with the argon ion laser inefficient [21, 34]. of RelyX ARC, regardless of the light curing source. ThisIn this study, the argon ion laser, working with the same may be explained by the chemical reaction that normallyenergy density as the QTH light, achieved an inadequate occurs between benzoyl peroxide and the tertiary aminedegree of conversion of Panavia F alone, due to the offset present in the composite material. If the tertiary aminenarrower spectral peak at about 488 nm, which could not supply is lower than the benzoyl peroxide content, theinitiate the photoinitiators present in this cement under the reaction cannot initiate, and the degree of conversionresin composite disk. When used with ED Primer, Panavia remains undisturbed . However, ED Primer is a systemF cured with argon ion laser did not display a significantly that contains a tertiary amine/benzoyl peroxide system,different degree of monomer conversion than that cured providing a complete self-cure reaction that could havewith the QTH or LED. For RelyX ARC there was no improved the physical properties of Panavia F when mixeddifference in the degree of conversion between the curing with this resin cement . For Panavia F, a primer A and Blights, indicating that the argon ion laser is suitable for mixture incorporated with the cement increased the degreecementing of indirect restorations, similar to the QTH and of conversion when the LED and the argon ion laser wereLED lights, when this material is used. used; whereas a similar degree of conversion was obtained For the photoactivation procedure, a resin composite disk when the QTH curing light was used. So for Panavia F, thewas prepared to simulate an indirect restoration, which is able ED Primer is essential for maintaining a satisfactory degreeto provide adequate physical and mechanical cement proper- of monomer conversion when cured with the light sourcesties . It is important to simulate a clinical situation most frequently used in clinical practice.representative of cementing an indirect restoration, since For indirect esthetic restorations, light plays an importantlight would be attenuated by the composite [2, 5] or ceramic role in promoting satisfactory conversion of the resin[17, 26, 35, 36], and the degree of cure might be lower than cement, ensuring adequate cementation [2, 5]. However,with direct curing. Besides, the resin luting thickness was the attenuation of the irradiance by ceramic or resin indirect0.5 mm, which is close to that seen in clinical situations, and restorations with a 2-mm thickness is such that only a halfit allowed satisfactory measurement by FTIR [1, 5]. Some of the irradiance reaches the resin cement beneath thesestudies [26, 30] used specimens with a cement thickness of materials [5, 39]. For metallic crowns, the chemical curingabout 1–2 mm, which is not clinically acceptable, as it may and incorporation of the catalyst into the resin lutingresult in a lower degree of conversion at the bottom of the cement might compensate for the total attenuation of thesample due to the depth of cure of the resinous material [21, curing light, since that would cause an effect only around30] and differences in the light curing irradiance that reaches the margin. Thus, clinicians should incorporate the chemicalall surfaces of the composite [14, 37]. catalyst into the manipulation of resin cements, since it The resin cements were activated totally by dual curing. improves or does not affect the degree of conversion of theseThe chemical curing of the luting materials with incorpo- luting materials.ration of the chemical catalyst was not tested because theresults of some studies have shown that chemical curingalone does not promote an adequate degree of conversion Conclusionof resin cements [2, 5]. On the other hand, manymanufacturers state that resin cement photoactivation may Based on these results, it can be concluded that the argonbe delayed for 5 or 10 minutes, since important chemical ion laser, LED, and QTH light promote an adequate degree
150 Lasers Med Sci (2012) 27:145–151of conversion for RelyX ARC, regardless of the 15. Alonso RCB, Cunha LG, Correr GM, Puppin-Rontani RM, Correr-Sobrinho L, Sinhoreti MAC (2006) Marginal adaptationaddition of the chemical catalyst. Nevertheless, Panavia of composite restorations photoactivated by LED, plasma ARCF, when photocured with the LED or argon ion laser, and QTH light using low modulus resin liners. J Adhes Dentshould be mixed with the chemical catalyst (ED Primer) 8:223–228to achieve a satisfactory degree of conversion, especially 16. Jandt KD, Mills RW, Blackwell GB, Ashworth SH (2000) Depth of cure and compressive strength of dental compositesin situations affected by the attenuation of light. Thus, cured with blue light emitting diodes (LEDs). Dent MatPanavia F should be used with the incorporation of the 16:41–47ED Primer on manipulation and photocured with a QTH 17. Ozturk N, Usumez A, Usumez S, Ozturk B (2005) Degree oflight unit. conversion and surface hardness of resin cement cured with different curing units. Quintes Int 36:771–777 18. Knezevic A, Tarle Z, Meniga A, Sutalo J, Pichler G, Ristic MAknowledgments We are grateful to CAPES for supporting this (2001) Degree of conversion and temperature rise duringstudy and to William Cunha Brandt for his scientific contribution. polymerization of composite resin samples with blue diodes. J Oral Rehab 28:586–591 19. Khosroshahi ME, Atai M, Nourbakhsh MS (2008) Photopolyme-References rization of dental resin as restorative material using an argon laser. Lasers Med Sci 23:399–406 20. Cassoni A, Ferla JO, Shibi JA, Kawano Y (2008) Knoop 1. Bandeca MC, El-Mowafy O, Saade EG, Rastelli ANS, Bagnato VS, microhardness and FT-Raman spectroscopic evaluation of a Porto-Neto ST (2009) Changes on degree of conversion of dual-cure resin-based dental material light-cured by an argon ion laser luting light-cured with blue LED. Laser Phys 19:1050–1055 and halogen lamp: an in vitro study. Photomed Laser Surg 2. Faria-e-Silva AL, Moraes RR, Ogliari FA, Piva E, Martins LRM 26:531–539 (2009) Panavia F: the role of the primer. J Oral Sci 51:255–259 21. Rode KM, Freitas PM, Lloret PR, Powell LG, Turbino ML (2009) 3. Cunha LG, Alonso RCB, Pfeifer CSC, Correr-Sobrinho L, Micro-hardness evaluation of a micro-hybrid composite resin Ferracane JL, Sinhoreti MAC (2008) Contraction stress and cured with halogen light, light-emitting diode and argon ion laser. physical properties development of a resin-based composite Lasers Med Sci 24:87–92 irradiated using modulated curing methods at two C-factors 22. Fleming M, Mailet W (1999) Photopolymerization of composite levels. Dent Mater 24:392–398 using the argon laser. Clin Prac 65:447–450 4. Alonso RCB, Cunha LG, Pantoja CAS, Puppin Rontani RM, Sinhoreti 23. Kelsey WP, Powell GL, Blankenau RJ, Whisenat BK (1989) MAC (2007) Modulated curing methods – effect on marginal and Enhancement of physical properties of resin restorative internal gap formation of restorations using different restorative materials by laser polymerization. Lasers Surg Med 9:623– composites. J Biomed Mat Res B Appl Biomat 82:346–351 627 5. Arrais CAG, Rueggeberg FA, Waller JL, De Goes MF, Giannini 24. Cassoni A, Youssef MN, Prokopowitsch I (2005) Bond strength M (2008) Effect of curing mode on the polymerization character- of a dentin bonding system using two techniques of polymeriza- istics of dual-cured resin cement systems. J Dent 36:418–426 tion: visible-light and argon ion laser. Photomed Laser Surg 6. Ferracane JL (1985) Correlation between hardness and degree of 23:493–497 conversion during the setting reaction of unfilled dental restorative 25. Conrado L, Munin E, Zangaro R (2004) Root apex sealing with resins. Dent Mat 1:11–14 different filling materials photopolymerized with fiber optic 7. Rueggeberg FA, Craig RG (1988) Correlation of parameters used delivered argon laser light. Lasers Med Sci 19:95–99 to estimate monomer conversion in a light-cured composite. J 26. Ozyesilag AG, Usumeza A, Gunduz B (2004) The efficien- Dent Res 67:932–937 cy of different light sources to polymerize composite 8. Ferracane JL, Mitchem JC, Condon JR, Todd R (1997) Wear and beneath a simulated ceramic restoration. J Prosthet Dent marginal breakdown of composites with various degrees of cure. J 91:151–157 Dent Res 76:1508–1516 27. Lu H, Stansbury JW, Bowman CN (2005) Impact of curing 9. Pearson GL, Longman CM (1989) Water sorption and solubility protocol on conversion and shrinkage stress. J Dent Res of resin-based materials following inadequate polymerization by a 84:822–826 visible-light curing system. J Oral Rehab 16:57–61 28. Schneider LFJ, Consani S, Sakagushi RL, Ferracane JL (2009)10. Faria-e-Silva AL, Arias VG, Soares LE, Martin AA, Martins LR Alternative photoinitiator system reduces the rate of stress (2007) Influence of fiber-post translucency on the degree of development without compromising the final properties of dental conversion of a dual-cured resin cement. J Endod 33:303–305 composite. Dent Mat 25:566–57211. Peutzfeldt A (1995) Dual-cure resin cements: in vitro wear and 29. Arikawa H, Takahashi H, Kanie T, Ban S (2009) Effect of various effect of quantity of remaining double bonds, filler volume and visible light photoinitiators on the polymerization and color of light curing. Acta Odontol Scand 53:29–34 light-activated resins. Dent Mat J 28:454–46012. Knezevic A, Ristic M, Demoli N, Tarle Z, Music S, Negovetic 30. Vrochari AD, Eliades G, Hellwig E, Wrbas K (2009) Curing Mandic V (2007) Composite photopolymerization with diode efficiency of four self-etching, self-adhesive resin cements. Dent laser. Oper Dent 32:279–284 Mat 25:1104–110813. Cunha LG, Alonso RCB, Souza-Junior EJC, Neves ACEC, 31. Cunha LG, Alonso RCB, Neves AC, De Goes MF, Ferracane JL, Correr-Sobrinho L, Sinhoreti MAC (2008) Influence of the curing Sinhoreti MAC (2009) Degree of conversion and contraction method on the post-polymerization shrinkage stress of composite stress development of a resin composite irradiated using halogen resins. J Appl Oral Sci 16:266–270 and LED at two C-factor levels. Oper Dent 34:24–3114. Cunha LG, Alonso RCB, Pfeifer CSC, De Goes MF, Ferracane 32. Powell GL, Blankenau RJ (2000) Laser curing of dental materials. JL, Sinhoreti MAC (2009) Effect of irradiance and light source on Dent Clin N Am 44:923–930 contraction stress, degree of conversion and push-out bond 33. Veheyen P (2001) Photopolymerization with the argon laser. J strength of composite restoratives. Am J Dent 22:165–170 Oral Laser Appl 1:49–54
Lasers Med Sci (2012) 27:145–151 15134. Hammesfahr PD, O’Connor MT, Wang X (2002) Light-curing 37. Jung H, Friesl KH, Hiller KA, Furch H, Bernhart S, Schmalz G technology: past, present and future. Compend Cont Educ Dent (2006) Polymerization efficiency of different photocuring units 23:18–24 through ceramic discs. Oper Dent 31:68–7735. Lee IB, An W, Chang J, Um CM (2008) Influence of 38. Arrais CAG, Giannini M, Rueggeberg FA (2009) Effect of sodium ceramic thickness and curing mode on the polymerization sulfinate salts on the polymerization characteristics of dual-cured shrinkage kinetics of dual-cured resin cements. Dent Mat resin cement systems exposed to attenuated light-activation. J Dent 24:1141–1147 37:219–22736. Meng X, Yoshida K, Atsuda M (2008) Influence of ceramic 39. Morais RR, Brandt WC, Naves LZ, Correr-Sobrinho L, Piva E thickness on mechanical properties and polymer structure of (2008) Light- and time-dependent polymerization of dual-cured resin dual-cured resin luting agents. Dent Mat 24:594–599 luting agent beneath ceramic. Acta Odontol Scand 66:257–261